A composition and size controllable approach for Au-Ag alloy nanoparticles
© Sun et al.; licensee Springer. 2012
Received: 3 November 2011
Accepted: 3 March 2012
Published: 18 April 2012
A capillary micro-reaction was established for the synthesis of Au-Ag alloy nanoparticles (NPs) with a flexible and controllable composition and grain size by tuning the synthesis temperature, the residence time, or the mole ratio of Au3+:Ag+. By extending the residence time from 5 to 900 s, enhancing the temperature from 120°C to 160°C, or decreasing the mole ratio of Au3+:Ag+ from 1:1 to 1:20, the composition of samples was changed continuously from Au-rich to Ag-rich. The particles became large with the increase of the residence time; however, synthesis temperatures showed less effect on the particle size change. The particle size of the Au-Ag alloy NPs with various composition could be kept by adjusting the mole ratio of Au3+:Ag+. TEM observation displayed that the as-obtained NPs were sphere-like with the smallest average size of 4.0 nm, which is half of those obtained by the traditional flask method.
KeywordsAu-Ag alloy Nanoparticles Composition Size Micro-reaction method
During the past decades, Au-Ag alloy has attracted great attentions due to its unique optical[1, 2], electronic, and catalytic properties. Especially, Au-Ag alloy displayed a comparable reduced reaction temperature when applied on CO oxidation in fields such as vehicle emissions, industrial waste, and the indoor atmosphere. Comparing with the traditional Au nanoparticles (NPs), Au-Ag alloy NPs showed a strong catalytic performance because of the synergistic effect of Au and Ag[5–8]. However, the synthesis of Au-Ag alloy NPs with mono-dispersed grain size, precise composition, and high surface activity is still a great challenge.
Several methods have been conducted on the synthesis of Au-Ag alloy, including laser ablation[9, 10], phase-transfer, digestive ripening, co-reduction of Au and Ag salts[13, 14], and galvanic replacement reaction. Most of the reported methods relied on complex process, high cost, and strong ligands. The co-reduction was regarded as a suitable method due to the Au-Ag NPs’ application preferability[13, 16, 17]. Wang et al. found such products with the smallest size as 8 nm obtained in flask could achieve a complete conversion of CO at 150°C, while Au catalyst was previously tested inactive up to 300°C.
The micro-reaction system has some attractive advantages including high control accuracy, superior size and shape controllability, no inert atmosphere protection, and fast reaction rate. Lin et al. got Ag NPs with the smallest size of 5.6 nm by a continuous flow micro-reactor. Wagner and Köhler and Köhler et al.[22–24] obtained Au NPs with the mean diameter between 24 nm and 35 nm in a chip micro-reactor. The size of the Ag and Au NPs was often tuned by changing the flow rate which was suitable for synthesizing mono-metal NPs, but not for bimetal NPs because of the variation of composition. Then, they synthesized star-like and sphere-like core-shell Au-Ag NPs with the average size between 80 nm and 120 nm in micro-fluidic systems by two or three steps; recently, a two-step micro-continuous flow-through method was used to synthesize multi-shell Au/Ag/Au NPs with the average size of 46.4 nm. However, Au-Ag alloy NPs with controlled size and composition are synthesized via micro-reaction, which has not been reported.
In this paper, the polytetrafluoroethylene (PTFE) capillary micro-reactor was adopted to synthesize Au-Ag alloy NPs where oleylamine (OLA) and octadecene (ODE) were taken as reductant and surfactant. The process parameters were systematically investigated. The composition and micro-structure of Au-Ag alloy NPs were deduced on the basis of the color of Au-Ag colloid. The structure, composition, and morphology were further studied by ultraviolet–visible spectrum (UV–vis), energy-dispersive spectrum (EDS), and transmission electron microscope (TEM).
Materials and set-up
Oleylamine (Aladdin Reagent Inc., Shanghai, People’s Republic of China), octadecene (Aladdin Reagent Company, Inc.), silver nitrate (AgNO3, Aladdin Reagent Inc.), chlorauric acid (HAuCl4·3H2O, Aladdin Reagent Inc.), ethanol (Aladdin Reagent Inc. and Sinopharm Chemical Reagent Co. Ltd., Shanghai, People’s Republic of China), and chloroform (Aladdin Reagent Inc. and Sinopharm Chemical Reagent Co. Ltd.) were used directly without further treatment. In our experiment, the capillary micro-reaction which was previously applied in the preparation of quantum dots was used to synthesize of Au-Ag NPs[25–28]. The syringe pump supplied a different flow rate which led to a variety of residence time. The blender and oil bath supported a stable temperature condition. The PTFE micro-reactor capillary (inside diameter: 750 μl; length: 100 cm), which is stable in the chemical reagents and can withstand moderate temperatures (up to 350°C), was coiled in oil bath. The structure of capillary enhanced the mass and heat transfer; moreover, it saved the space. Au-Ag colloid was collected in a collector and, then, separated by centrifuge (8,000 rpm, 10 min). The average size distribution of Au-Ag alloy was obtained by the statistical calculation of more than 150 particles from different parts of the grid.
Characterization of the Au-Ag alloy NPs
EDS was applied to determine the mole ratio of Au and Ag using a scanning electron microscope (JSM-6360LV, JEOL, Tokyo, Japan) equipped with EDX (FALCON, EDAX, Kanagawa, Japan). Ultraviolet visible spectrum (UV–vis) analysis was carried out on a spectrophotometer (Cary 50, Varian Medical Systems, Inc., Tokyo, Japan). Chloroform was used as a standard for the background correction. The relationship between the composition of the Au-Ag NPs and absorption wavelength was investigated by UV–vis absorption spectra and EDS. A high-resolution transmission electron microscope (HR-TEM, JEM-2100 F, JEOL Ltd., Akishima, Tokyo, Japan) operated at 200 kV was used to observe the morphology. The sample for TEM was prepared by dipping an amorphous carbon-copper grid in a chloroform solution dispersed Au-Ag NPs homogeneously by sonicating for 5 min; then, the sample was left to evaporate in air at room temperature.
Results and discussion
Formation of Au-Ag alloy NPs
Figure1B presents the normalized UV–vis absorption spectra of the samples. We can clearly find that all Au-Ag samples display only one Abs. peak which blue-shifted from 489 to 432 nm with the increase of the residence time from 120 to 640 s. For the physical mixture of Au and Ag NPs, there are two Abs. peaks between 522 and 410 nm. When Au-Ag alloy was further added in, a third Abs. peak would show up, corresponding to a mixture of Au, Au-Ag alloy, and Ag. Inset of the Figure1B is the plot of the Abs. peaks against the Au mole ratio of various Au-Ag alloy NPs obtained from EDS, which manifested almost a linear relationship. It is commonly confirmed of a Au-Ag alloy formation when UV–vis absorption spectra show only one Abs. peak, and the Abs. peak against the mole ratios of Au exhibits a linear fashion[12, 31, 33].
At higher temperature, the Au-Ag NPs may be a mixture of Au-Ag alloy, Ag or Au. As shown in the inset of Figure2, the plot of Abs. peak against the Au mole ratio of various Au-Ag alloy NPs displays an almost a linear relationship, which implies Au-Ag alloy can also be synthesized at 160°C.
It can be seen from Figure3 insets (b) and (c) that the ideal linear fashions between the Abs. peak and the Au mole ratio of various Au-Ag alloy NPs are shown, which confirm the Au-Ag alloy NPs that were synthesized with the mole ratio changed from 1:5 to 1:50 at 140°C.
Grain size control
The synthesis temperature often has a strong effect on the size of NPs. Figure5 D, E, F line exhibits the relationship between average particle size of Au-Ag alloy NPs and synthesis temperature. Samples D, E, and F prepared at different temperatures (120°C, 140°C, and 160°C, respectively) during different residence times (40, 15, and 8 s, respectively) have the same composition (509 nm), and the average sizes are 4.0, 4.0, and 4.1 nm, respectively. Here, the little change of size indicates the Au-Ag alloy of the same composition, and size can be achieved at a shorter residence time by enhancing the temperature from 120°C to 160°C.
The spherical Au-Ag alloy NPs with controllable composition and size were synthesized by a simple capillary micro-reaction method. The composition of Au-Ag alloy NPs could be tuned by controlling the synthesis conditions. The Abs. peak of Au-Ag alloy blue-shifted via enhancing the synthesis temperature, increasing the residence time, or decreasing the mole ratio of Au3+:Ag+. The Au-Ag alloy with the same composition and similar size could be obtained by enhancing the temperature from 120°C to 160°C, while the residence time got shorter. The Au-Ag alloy NPs changed from Au-rich to Ag-rich by increasing the residence time, corresponding with a growth of particle size. The size with different composition could be controlled as 4 nm by adjusting the mole ratio of Au3+:Ag+. Thus, micro-reaction provided a suitable and flexible way for producing composition and size-controlled Au-Ag alloys.
- Abs. peak:
high-resolution transmission electron microscope
transmission electron microscope
Authors appreciated the financial supports from the Fundamental Research Funds for National Nature Science Foundation of China (51172072), the Fundamental Research Funds for the Central Universities (WJ0913001), the Focus of Scientific and Technological Research Projects (109063), and the State Key Laboratory of Chemical Engineering at ECUST (SKL-ChE-08 C09).
- Broyer M, Cottancin E, Lerme J, Pellarin M, Fatti ND, Vallee F, Burgin J, Guillon C, Langot P: Optical properties and relaxation processes at femtosecond scale of bimetallic clusters. Faraday Discuss 2008, 138: 137–145.View Article
- Gu XF, Qiu T, Zhang WJ, Chu PK: Light-emitting diodes enhanced by localized surface plasmon resonance. Nanoscale Res Lett 2011, 6: 199–210. 10.1186/1556-276X-6-199View Article
- Lee KS, EI-Sayed MA: Gold and silver nanoparticles in sensing and imaging: sensitivity of plasmon response to size, shape, and metal composition. J Phys Chem B 2006, 110: 19220–19225. 10.1021/jp062536yView Article
- Mitsudome T, Mikami Y, Funai H, Mizugaki T, Jitsukawa K, Kaneda K: Oxidant-free alcohol dehydrogenation using a reusable hydrotalcite-supported silver nanoparticles catalyst. Angew Chem Int Ed 2008, 47: 138–141. 10.1002/anie.200703161View Article
- Zemichael FW, Al-Musa A, Cumming IW, Hellgardt K: Propene partial oxidation over Au-Ag alloy and Ag catalysts using electrochemical oxygen. Solid State Ionics 2008, 179: 1401–1404. 10.1016/j.ssi.2008.03.011View Article
- Chaki NK, Tsunoyama H, Negishi Y, Sakurai H, Tsukuda T: Effect of Ag-doping on the catalytic activity of polymer-stabilized Au clusters in aerobic oxidation of alcohol. J Phys Chem C 2007, 111: 4885–4888. 10.1021/jp070791sView Article
- Liu J-H, Wang A-Q, Chi Y-S, Lin H-P, Mou C-Y: Synergistic effect in an Au-Ag alloy nanocatalyst: CO oxidation. J Phys Chem B 2005, 109: 40–43.View Article
- Alberto S, Antonio A, Catherine L, Agnes T, Rodolfo Z: Bimetallic Au-Ag/TiO2 catalyst prepared by deposition-precipitation: high activity and stability in CO oxidation. J Catal 2011, 281: 40–49. 10.1016/j.jcat.2011.04.003View Article
- Lee I, Han SW, Kim K: Production of Au-Ag alloy nanoparticles by laser ablation of bulk alloys. Chem Commun 2001, 18: 1782–1783.View Article
- Jafarkhani P, Torkamany MJ, Dadras S, Chehrghani A, Sabbaghzadeh J: Necklace-shaped Au-Ag nanoalloys: laser-assisted synthesis and nonlinear optical properties. Nanotechnology 2011, 22: 235703. 10.1088/0957-4484/22/23/235703View Article
- Hostetler MJ, Zhong CJ, Anderegg J, Gross SM, Evans ND, Porter M, Murray RW: Stable, monolayer-protected metal alloy clusters. J Am Chem Soc 1998, 120: 9396–9397. 10.1021/ja981454nView Article
- Link S, Wang ZL, EI-Sayed MA: Alloy formation of gold-silver nanoparticles and the dependence of the plasmon absorption on their composition. J Phys Chem B 1999, 103: 3529–3533. 10.1021/jp990387wView Article
- Wang C, Yin HF, Chan R, Peng S, Dai S, Sun SH: One-pot synthesis of oleylamine coated AuAg alloy NPs and their catalysis for CO oxidation. Chem Mater 2009, 21: 433–435. 10.1021/cm802753jView Article
- Mallin MP, Murphy CJ: Solution-phase synthesis of sub-10 nm Au-Ag alloy nanoparticles. Nano Lett 2002, 2: 1235–1237. 10.1021/nl025774nView Article
- Zhang QB, Lee JY, Yang J, Boothroyd C, Zhang JX: Size and composition tunable Au-Ag alloy nanoparticles by replacement reactions. Nanotechnology 2007, 18: 245605–245612. 10.1088/0957-4484/18/24/245605View Article
- Peng XG, Manna L, Yang WD, Wickham J, Scher E, Kadavanich A, Alivisatos AP: Shape control of CdSe nanocrystals. Nature 2000, 404: 59–61. 10.1038/35003535View Article
- Burda C, Chen XB, Narayanan R, EI-Sayed MA: Chemistry and properties of nanocrystals of different shapes. Chem Rev 2005, 105: 1025–1102. 10.1021/cr030063aView Article
- Qian K, Huang WX, Jiang ZQ, Sun HX: Anchoring highly active gold nanoparticles on SiO2 by CoOx additive. J Catal 2007, 248: 137–141. 10.1016/j.jcat.2007.02.010View Article
- Nightingale MA, Mello JC: Microscale synthesis of quantum dots. J Mater Chem 2010, 20: 8454–8463. 10.1039/c0jm01221aView Article
- Lin XZ, Terepka AD, Yang H: Synthesis of silver nanoparticles in a continuous flow tubular microreactor. Nano Lett 2004, 4: 2227–2232. 10.1021/nl0485859View Article
- Wagner J, Köhler JM: Continuous synthesis of gold nanoparticles in a microreactor. Nano Lett 2005, 5: 685–691. 10.1021/nl050097tView Article
- Köhler JM, Romanus H, Hübner U, Wagner J: Formation of star-like and core-shell AuAg nanoparticles during two- and three-step preparation in batch and in microfluidic systems. J Nanomate 2007, 2007: 98134–98140.
- Köhler JM, Held M, Hübner U, Wagner J: Formation of Au/Ag nanoparticles in a two step micro flow-through process. Chem Eng Technol 2007, 30: 347–354. 10.1002/ceat.200600388View Article
- Knauera A, Thetea A, Lia S, Romanus H, Csáki W, Fritzsche W, Köhler JM: Au/Ag/Au double shell nanoparticles with narrow size distribution obtained by continuous micro segmented flow synthesis. Chem Eng J 2011, 166: 1164–1169. 10.1016/j.cej.2010.12.028View Article
- Luan WL, Yang HW, Tu S-T: Synthesis of efficiently green luminescent CdSe/ZnS nanocrystals via microfluidic reaction. Nanoscale Res Lett 2008, 3: 134–139. 10.1007/s11671-008-9125-5View Article
- Luan WL, Yang HW, Tu S-T, Wang ZM: Open-to-air synthesis of monodisperse CdSe NCs via microfluidic reaction and its kinetics. Nanotechnology 2007, 18: 175603–175608. 10.1088/0957-4484/18/17/175603View Article
- Wan Z, Yang HW, Luan WL, Tu S-T: Facile synthesis of monodisperse CdS nanocrystals via microreaction. Nanoscale Res Lett 2010, 5: 130–137. 10.1007/s11671-009-9454-zView Article
- Tu S-T, Yu XH, Luan WL, Loewe H: Development of micro chemical, biological and thermal systems in China. Chem Eng J 2010, 163: 165–179. 10.1016/j.cej.2010.07.021View Article
- Angshuman P, Sunil S, Surekha D: Synthesis of Au, Ag and Au-Ag alloy nanoparticles in aqueous polymer solution. Colloids Surf A 2007, 302: 51–57. 10.1016/j.colsurfa.2007.01.054View Article
- Sun YG, Xia YN: Mechanistic study on the replacement reaction between silver nanostructures andchloroauric acid in aqueous medium. J Am Chem Soc 2004, 126: 3892–3901. 10.1021/ja039734cView Article
- Poovathinthodiyi R, Jie F, Scoot LW: A simple and “green” method for the synthesis of Au, Ag, and Au-Ag alloy nanoparticles. Green Chem 2006, 8: 34–38. 10.1039/b512540eView Article
- Devarajan S, Bera P, Sampath S: Bimetallic nanoparticles: a single step synthesis, stabilization, and characterization of Au-Ag, Au-Pd, and Au-Pt in sol–gel derived silicates. J Colloid Interf Sci 2005, 290: 117–129. 10.1016/j.jcis.2005.04.034View Article
- Chen HM, Liu RS, Jang L-Y, Lee J-F, Hu SF: Characterization of core-shell type and alloy Ag/Au bimetallic clusters by using extended X-ray absorption fine structure spectroscopy. Chem Phy Lett 2006, 421: 118–123. 10.1016/j.cplett.2006.01.043View Article
- Yu H, Chen M, Rice PM, Wang SX, White RL, Sun S: Dumbbell-like bifunctional Au-Fe3O4 nanoparticles. Nano Lett 2005, 5: 379–382. 10.1021/nl047955qView Article
- Chen M, Feng Y-G, Wang X, Li T-C, Zhang J-Y, Qian DJ: Silver nanoparticles capped by oleylamine: formation, growth, and self-organization. Langmuir 2007, 23: 5296–5304. 10.1021/la700553dView Article
- Yang J, Lee JY, Too H-P: Core-shell Ag-Au nanoparticles from replacement reaction in organic medium. J Phys Chem B 2005, 109: 19208–19212. 10.1021/jp052242xView Article
- Liz-Marzán LM, Philipse AP: Synthesis and optical properties of gold-labeled silica particles. J Colloid Interf Sci 1995, 176: 459–466. 10.1006/jcis.1995.9945View Article
- Chen DH, Chen CJ: Formation and characterization of Au-Ag bimetallic nanoparticles in water-in-oil microemulsions. J Mater Chem 2002, 12: 1557–1562. 10.1039/b110749fView Article
- Jiang XC, Chen WM, Chen CY, Xiong SX, Yu AB: Role of temperature in the growth of silver nanoparticles through a synergetic reduction approach. Nanoscale Res Lett 2011, 6: 32–40.
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.